Presentation on theme: "Nanoimprint lithography (NIL)"— Presentation transcript:
1 Nanoimprint lithography (NIL) Overview.Thermal NIL resists.Residual layer after NIL.NIL for large features (more difficult than small one).Room temperature NIL, reverse NIL, inking.NIL of bulk resist (polymer sheet, pellets).ECE 730: Fabrication in the nanoscale: principles, technology and applicationsInstructor: Bo Cui, ECE, University of Waterloo;Textbook: Nanofabrication: principles, capabilities and limits, by Zheng Cui
2 Nanoimprint lithography: patterning by mechanical replication moldsubstrate
3 Two NIL approaches Thermal NIL UV-curable NIL UV-light RIE residual layer, transfer into under-layerRIE residual layerHeat up to soften the resist, imprint, cool down and separateLiquid (soft) resist, hardened by UV irradiation due to cross-linking
4 Printing: some history During , Bi Sheng invented movable type printing technique. Hardened clay as mold.12th century metal type printing techniques were developed in Korea.1450 Gutenberg introduced his press. 300 two-volume bibles printed.………1970´s compact disks (CD).1996, Nano-Imprint Lithography (NIL), sub-10 nm feature size, high throughput and low cost.Today, NIL is one candidate (though not top candidate) for next-generation lithography for IC industry.The bottom line is, NIL has the highest resolution (sub-5nm) and is fast. It will come into play when no other lithography can do the job.Gutenberg bible (1450)Duplicated by NIL (2000)
5 NIL not ready yet for ICs, but never excluded ML2: maskless lithography (EBL, SPM..)ITRS (2006) Projections for Lithography Technology
6 Comparison between thermal and UV NIL Resist materialThermoplastic or thermal-set(i.e. cured upon heating)UV-sensitive monomerplus various additivesResolutionSub-5nm2nm demonstrated, but volume shrinkage after cross-linkingTemperature30-100oC above TgRoom temperaturePressureNormally over 10 bar~ 1 bar, or higherResist applicationSpin coating, easySpin coating or dropResist thicknessUp to many m,easy for pattern transferTypically < 100nm,need an extra transfer layerCycle time1-30 min, slow~1 minLarge features~100 m, difficultRelatively easy, low viscosityAlignment~ 1 m, difficult; CTE mismatch20nm demonstratedApplicationBroad range, simple and work with many materialsTargeted for semiconductor industry with alignmentTg: glass transition temperatureCTE: coefficient of thermal expansion
8 Key advantage of NIL: highest resolution Sub-5 nm features and 14nm pitch nanoimprintYet, feature size and pitch still limited by mold making. They can go smaller.No more light diffraction limit, charged particles scattering, proximity effect…Sub-10nm feature size, over a large area with high throughput and low cost.
9 Another key advantage: 3D imprinting 3D moldPatterning of the via and interconnect layers simultaneously, in CMOS BEOL .Potentially reduces the number of masking levels needed in BEOL.(BEOL: back end of line)Wikipedia: Back end of line (BEOL) is the portion of integrated circuit fabrication line where the active components (transistors, resistors, etc.) are interconnected with wiring on the wafer. BEOL generally begins when the first layer of metal is deposited on the wafer. It includes contacts, insulator, metal levels, and bonding sites for chip-to-package connections.
10 Imprinting in presence of a dust particle Dust is one of the most serious problem for NIL, defect area>>>>>dust size.To prevent mold wafer breaking, sandwich the mold/substrate stack with something soft, such as a paper or plastic.
11 Nanoimprint lithography (NIL) Overview.Thermal NIL resists.Residual layer after NIL.NIL for large features (more difficult than small one).Room temperature NIL, reverse NIL, inking.NIL of bulk resist (polymer sheet, pellets).
12 Desired resist properties Good adhesion to the substrate, uniform film thickness, easy spinning.High pattern transfer fidelity, no adhesion to the mold during seperation.Low viscosity during imprinting.Low imprint pressure and temperature.But sufficient thermal stability in subsequent processes, e.g. RIE, lift-off.High plasma etch resistance for pattern transfer into under-layers.Soluble in non-toxic solvents, deposition by spin-coating.Minimal shrinkage (for UV and thermal curable resist).Mechanical strength and tear resistance.
13 How much initial material (resist) is needed? Polymer is not compressible, so conservation of volume.Too thick h0 leads to large hf, difficult for pattern transfer.Too thin h0 increases mold wear and damage.Alternative Lithography: Unleashing the Potentials of Nanotechnology (book), 2003.
14 “Standard” resist for NIL: PMMA Glass transition and flow temperature of PMMATS: sub-transitionTG: glass transitionTF: flowHowever, PMMA is far away from being an ideal NIL resist. It is popular simply because people are familiar with it (since it is resist for many other lithographies).
15 Shear modulus of different molecular weight PMMAs Flow temperature of PMMA (and other amorphous polymers) increases with increasing molecular weight.Comments:PMMA is the choice for beginners, not optimized for NIL. Tg=105oC, NIL at >150oC.Polystyrene (Tg close to PMMA) is slightly better – easy separation due to lower surface energy.Poly(vinyl phenyl ketone) is comparable to polystyrene but with Tg only 58oC. NIL at 95oC.
16 Another thermal NIL resist: TOPAS polymers TOPAS: Cyclic olefinic copolymer (norbornene and ethylene)Attractive properties:– very un-polar– very low water absorption– high optical transparency (>300 nm)– high chemical resistance– low surface energy– high plasma etch resistanceBut finding solvent system giving homogeneous and stable solutions is not an easy task (chemical resistance, hard to dissolve)Applications: lab-on-a-chip micro-fluidic system…Commercial Topas solutions: (from Micro-Resist)mr-I T85 with Topas grade 8007mr-I T65 with Topas grade 9506Similar product: Zeonor from Zeon or Zeonex
17 Tg can be lowered by adding plasticizer into the resist no plasticizer+ plasticizer+ lots plasticizerplasticizerPlasticizer: decreased chain entanglementincreased chain motionPlasticizer: monomers, solvents, small molecules
18 Polymer with low Tg Low imprint temperature Good polymer flow at moderate temperatureLess problems with thermal expansionShorter cycle time due to faster reaching the imprint temperature (?)Not always, cooling to ambient temperature takes long time, not heating.Example: thermoplastic with Tg 40 °CLeft: 400 nm lines and trenches: immediately after imprinting Right: same patterns after heating the imprint to 60°C for 5min.Thermal stability of imprinted patterns (deterioration by thermal flow) is determined by the glass transition temperature.Sufficient thermal stability of imprinted patterns is necessary in subsequent processes such as metal evaporation for liftoff or plasma etching.
19 If Tg is too low…10 days after imprinting a low Tg resist
20 Approach to thermal stability Thermal-set/curable resist: polymer is cured (cross-linked) upon heating, making it stable at very high temperatures.
21 Thermal and photochemical curing Cured polymerLinear or branched thermoplastic(pre)polymerCuring:Cross-linking of the macromolecules, generation of a spatial macromolecular network.
23 Fast iso-thermal nanoimprint lithography (NIL without thermal cycle) Isothermal imprinting due to increase in Tg during imprinting.Reduce issues of thermal expansion.Decrease considerably imprint time (since no cooling).Starting model system:Best imprint results (no displacement of patterns) when mold is detached at imprint temperature (i.e. no cooling).NIL at 190oC for 1 hour (sufficient curing) necessary for excellent patternsAdd initiator A + plasticizer 1:Imprint at 100oC for 10min, no cooling.Film thickness 170nm, 100nm trenches, 10-20nm residual layer.(Initiator to increase curing speed; plasticizer to lower imprint temperature)
24 Functional resist: nano-crystal(NC)/polymer based materials Synthesis and functionalisation of colloidal nano-particles for incorporation into thermoplastic or thermal-curing (i.e. thermal-set) polymers.Tuning of functional properties:Optical absorption and emissionMechanical StabilityConductivityProcessability…Size dependent luminescent CdSe NCs (quantum dot)
25 Imprinting on luminescent nano-crystal/PMMA based co-polymer composites Under illuminationNo illuminationnano-crystals (NC) in PMMA modified co-polymer.Homogeneous distribution of NCs inside the polymer matrix.
26 Functional “resist”: semiconducting polymer SEM image of 200nm period MEH-PPV grating R-P3HT grating with 200nm period1 mMEH-PPV Tg=65oC.Hot embossing at 120oC and 20bar.MEH-PPV spun on a PEDOT/ITO/glass.R-P3HT 200nm period grating.NIL at 160oC and 35 bar.Strong physical bond, high transition temperature.
27 Nanoimprint lithography (NIL) Overview.Thermal NIL resists.Residual layer after NIL.NIL for large features (more difficult than small one).Room temperature NIL, reverse NIL, inking.NIL of bulk resist (polymer sheet, pellets).
28 Residual layer: thinner is better for easier pattern transfer RIESuch a tapered profile makes liftoff almost impossibleResistSubstrateToo thick residual layer makes subsequent RIE more demanding: hard to control profile, pattern size shrinkage (CD loss).So resist thickness should be pattern height of mold.CD: critical dimension.
29 How to get rid of residual layer Light-blocking metal layer, use a developer solution instead of the separate O2 RIE step.Comparison of residual layers in micro-scale resist pattern obtained by: (a) conventional NIL; (b) the current technique where no residual layer is left.Un-exposed area developed(since SU-8 is negative resist)Cheng and Guo, “A combined-nanoimprint-and-photolithography patterning technique”, MEE, 2004.
30 ICP etching of residue layer ICP: inductively coupled plasma, high plasma density and etching rate, better control(According to an ICP tool seller)ICP provides the best performance for etching residual layer:Low pressure processing minimizes isotropic (lateral) etching and loss of profile.Lower temperature processing also helps.Low bias processing minimizes faceting at the top of the lines.Polystyrene Nano-imprint descum (i.e. residue removal) on Al. 200nm residual removed in 2 minutes using a pure O2 ICP plasma – linewidth remains constant at 0.35μm (??)
31 Another way to reduce residue layer effect: use tri-layer (or bi-layer) resist Square (mm) imprinted into PMMAOptical imageProfileafter excessive etchBut for nanoscale features…Such a profile makes liftoff difficult.Solution: use tri-layer resist system200nm2mmSchematicmold waferresist need to etchTri-layer resistsilicon waferPMMAPMMAthinSiO2Need excessive etch to remove the thick resist at the square centerbottom polymer layer
32 Nanoimprint lithography (NIL) Overview.Thermal NIL resists.Residual layer after NIL.NIL for large features (more difficult than small one).Room temperature NIL, reverse NIL, inking.NIL of bulk resist (polymer sheet, pellets).
33 NIL for small features/high resolution (<10nm) Press liquid into a nano-holePressure (P)Thermal NIL into PMMA(10nm pillar array mold)F=2RSurface tension ()UV-curable NIL, 2nm carbon nanotube mold Pressure 1/diameter. But for protruded mold features (pillars…), local pressure at the pillar is much higher than average - easy to imprint.Hua … Rogers, “Polymer imprint lithography with molecular-scale resolution”, Nano Lett. 2004
34 NIL for large features (>100 m) - simultaneous pattern duplication of large and small features Application: large features are needed to connect small ones to the outside world (electrodes…).Challenge: more polymer must be displaced over longer distances.A popular approach: two-step process - small features by NIL, large ones by photolithography with alignment.Problems when both small and large features are presentSchematics of pattern failure mechanisms in NIL as a result of: (a) non-uniform pattern height; (b) non-uniform residual layer thickness; (c) incomplete nano-pattern replication.Cheng, “One-step lithography for various size patterns with a hybrid mask-mold”, Microelectronic Engineering 71, 288–293 (2004).
35 NIL pattern uniformity Etch some dummy holes/trenches hereThe fill factor should be kept constant: better flow and shorter imprint time.Different fill factor across mold leads to different sinking rates.Mold bending leads to non-uniform residual layer on substrate.One solution: fabricate dummy cavities/protrusions to create constant fill factor.
36 Combined UV (for macro) and nanoimprint lithography (for nano) hybrid mask-moldSU-8 is used both as a photo-resist and thermal NIL resist.(SU-8 is a photo-resist, but not a UV-NIL resist (hard to imprint at RT). Instead, it can be used as a thermal NIL resist, Tg50oC)Schematics of the technique by using a hybrid mask-mold for one-step lithography of both large- and nano-patternsSEM micrograph of resist patterns obtained by the technique with hybrid mask-mold.Cheng, “One-step lithography for various size patterns with a hybrid mask-mold”, Microelectronic Engineering 71, 288–293 (2004).
37 Modeling of liquid flow for large features (>>pattern depth) moldh0SubstrateLiquidAssumptions:Periodic mold structure (period 2L)Ignore inertial, gravitational forces and surface tensionResist film thickness = mold trench depth = h0L: achievable feature sizep: pressure: imprinting time: viscosityh0: film thickness
38 Strategy to imprint large features (mm) L: achievable feature sizep: pressure: melting time: viscosityFor thermoplastic polymer PMMA at T>TgMw: molecular weightn=1 for Mw<MC, un-entangled moleculesn=3.4 for Mw>MC, entangled moleculesViscosity for PMMA (Mc=30kg/mol)a) 12 kg/mol, 200oC; b) 12 kg/mol,150oC; c) 120 kg/mol, 200oCa:b:c=1:126:278Use low molecular weight PMMA and imprint at high temperature
39 Strategy to imprint large features (mm) Square (mm) imprinted into PMMAafter excessive etchBut for nanoscale features…Such a profile makes liftoff difficult.Solution: use tri-layer resist systembottom polymer layerPMMAthinSiO2Tri-layer resistOptical imageProfile200nm2mmSchematicmold waferresist need to etchsilicon waferNeed excessive etch to remove the thick resist at the square center
40 Fabrication process flow Moldtri-layer resistPMMASiO24. RIE ARC (O2 gas, etch little SiO2)ARCCrsilicon wafer1. ImprintARC:Anti-reflection coating, cross-linked polymer.5. Evaporate Cr2. RIE PMMA (excessive etch)6. Liftoff Cr (dissolve ARC)7. RIE Si (etch little Cr)3. RIE SiO2 (CHF3 gas)
41 Result 1.6mm square Line-width in the mold is 80nm Line-width in the duplicated pattern is 98nm50403098nmLine-width change (nm)1.3mm square201090120150180210240270PMMA etched (nm)(RIE PMMA 180nm)For small features, line-width increased by 18nm (acceptable).For large features, 1.3mm squares were faithfully duplicated.Cui and Veres, “Pattern replication of 100 nm to millimeter-scale features by thermal nanoimprint lithography”, MEE, 2006
42 Nanoimprint lithography (NIL) Overview.Thermal NIL resists.Residual layer after NIL.NIL for large features (more difficult than small one).Room temperature NIL, reverse NIL, inking.NIL of bulk resist (polymer sheet, pellets).
43 Room temperature (“thermal”) NIL RT-NIL process does not require a resist thermal cycle when pressing a mold onto the resist.Use special material, such as hydrogen silsequioxane (HSQ), or ultrahigh pressure.SOG: spin on glassMatsui, “Room-temperature nanoimprint and nanotransfer printing using hydrogen silsequioxane”, JVST B, 2003
44 Room temperature (“thermal”) NIL Pre-baking is important:HSQ has a high viscosity without prebaking.The effect of prebaking HSQ is to remove the solvent init.The hardness of HSQ increases at around 150°C (so don’t bake at higher T).“Nanoimprint and nanocontact technologies using hydrogen silsequioxane”, JVST B, 2005
45 NIL results into HSQ at RT 1 min press time by RT-NIL at 40atm pressure.Etch rate ratio for AZ photoresist to HSQ (like SiO2) is >100.
46 Reverse NIL and multi-dimensional patterning of polymer nanostructures Layer-by-layer NIL (repeated reverse NIL)L. J. Guo, J. Phys. D 37, R123 (2004)
47 Imprint by inking Inking process TTg Selectively Surface Treatment MoldInking processPDMS pad impregnated with medium surface energy filmSelectively Surface TreatmentProtrusions with medium surface energy treatmentSidewalls and trenches with lower surface energy treatmentTTgSpin coat polymer and annealingInk to substrateBao…Guo, “Polymer inking as a micro- and nanopatterning technique”, J. Vac. Sci. Tech. B, 2003, 21, 2749
48 Nanoimprint lithography (NIL) Overview.Thermal NIL resists.Residual layer after NIL.NIL for large features (more difficult than small one).Room temperature NIL, reverse NIL, inking.NIL of bulk resist (polymer sheet, pellets).
49 Hot embossing pellets Cheap setup V. Studer, A. Pépin, Y.Chen, Appl. Phys. Lett. 80, 3614 (2002)
50 Hot embossing PMMA pellets: results NIL at 180°C, 50bar pressure for 10 minFor fabricating micro- and nano-fluidic channels in thermoplastic polymers.
51 Hot embossing polystyrene pellets Polystyrene is bio-compatible (cell culturing Petri-dish is made of polystyrene perhaps plus some additives).4m period gratingcellgrating substrateApplication: contact guidance of cell growthDefinition: anisotropic topographic features induce cells to align along the direction of the anisotropy.Importance: in tissue engineering, if tissue is to be repaired, the new cells must be aligned and positioned correctly.
52 Tissue engineering: corneal and dermal cell growth Corneal cellDermal cellgratingDay 1first layerfirst layerDay 12second layerFirst layer: both cells aligned with the grating (as expected).Second layer:Corneal cells - oriented at 60° relative to first layer, as in a native corneaDermal cells - no orientation
Your consent to our cookies if you continue to use this website.